# Difference between revisions of "Flory-Huggins theory"

Line 24: | Line 24: | ||

Therefore: | Therefore: | ||

− | *Positive values of <math>\chi</math> necessarily lead to incompatibility for | + | *Positive values of <math>\chi</math> necessarily lead to incompatibility for polymer mixtures of high molecular weight. |

− | * | + | *Polymer mixing always take place if the <math>\chi</math> parameter is negative. Compatible polymer mixtures with negative <math>\chi</math> are due to specific interactions between given polymer segments. Compatibility can be induced by introducing opposite charges in the different polymers or by the presence of a copolymer containing A and B segments. |

*For a polymer solution, the critical Flory-Huggins parameter is close to <math>1/2</math>. | *For a polymer solution, the critical Flory-Huggins parameter is close to <math>1/2</math>. | ||

## Revision as of 14:43, 6 August 2008

The **Flory-Huggins theory** for solutions of polymers was developed by Maurice L. Huggins (Ref. 1) and Paul J. Flory (Ref. 2). The Flory-Huggins theory defines the volume of a polymer system as a lattice which is divided into small subspaces (called sites) of the same volume. In the case of polymer solutions, the solvent is assumed to occupy single sites, while each polymer chain occupies sites. The repulsive forces in the system are modelled by requiring each lattice site to be occupied by only a single segment. Attractive interactions between non-bonded sites are included at the lattice neighbour level. Assuming random and ideal mixing of two polymers, i.e. mixing volume , it is possible to obtain the well-known expression for the combinatorial entropy of mixing per site of the Flory Huggins theory,

where is the volume fraction of the component and is the number of segments in each type of polymer chain, and is the molar gas constant. Applying the concept of regular solutions and assuming all pair interactions in the framework of a mean-field theory yields for the enthalpy of mixing

where is the absolute temperature. According to the preceding equations, the Flory-Huggins equation can be expressed in terms of the Gibbs energy function of mixing for a binary system

where is the Flory-Huggins binary interaction parameter, defined as:

where is the net energy associated with two neighbouring lattice sites of the different polymer segments for the same type or for the different types of polymer chains. Although the theory considers as a fixed parameter, experimental data reveal that actually depends on such quantities as temperature, concentration, pressure, molar mass, molar mass distribution. From a theoretical point of view it may also depend on model parameters as the coordination number of the lattice and segment length.

For polymers of high molecular weight (i.e. ) the entropic contribution is very small and the miscibility or immiscibility of the system mainly depends on the value of the enthalpy of mixing. In this case, miscibility can only be achieved when is negative. Assuming a temperature-dependent parameter, T vs. phase-separation diagrams can be constructed. For long polymers, miscibility can only be achieved when . The parameter at the critical point can be obtained from the definition of the critical point and the Flory-Huggins expression for the free-energy of mixing. The result is

Therefore:

- Positive values of necessarily lead to incompatibility for polymer mixtures of high molecular weight.
- Polymer mixing always take place if the parameter is negative. Compatible polymer mixtures with negative are due to specific interactions between given polymer segments. Compatibility can be induced by introducing opposite charges in the different polymers or by the presence of a copolymer containing A and B segments.
- For a polymer solution, the critical Flory-Huggins parameter is close to .

The parameter is somewhat similar to a second virial coefficient expressing binary interactions between molecules and, therefore, it usually shows a linear dependence of

where and are assumed to be constants, but can actually depend on density, concentration, molecular weight, etc. A usual interpretation is that represents an enthalpic quantity and an entropic contribution, although both and are actually empirical parameters. According to this description, the systems should show an upper critical temperature. Many polymer systems and solutions, however, show an increase of for increasing temperatures (negative entropic contribution) what implies the existence of a lower critical temperature.